Abstract
The bulk photovoltaic effect (BPVE) refers to the generation of a steady photocurrent and abovebandgap photovoltage in a singlephase homogeneous material lacking inversion symmetry. The mechanism of BPVE is decidedly different from the typical p–n junctionbased photovoltaic mechanism in heterogeneous materials. Recently, there has been renewed interest in ferroelectric materials for solar energy conversion, inspired by the discovery of abovebandgap photovoltages in ferroelectrics, the invention of low bandgap ferroelectric materials and the rapidly improving power conversion efficiency of metal halide perovskites. However, as long as the nature of the BPVE and its dependence on composition and structure remain poorly understood, materials engineering and the realisation of its true potential will be hampered. In this review article, we survey the history, development and recent progress in understanding the mechanisms of BPVE, with a focus on the shift current mechanism, an intrinsic BPVE that is universal to all materials lacking inversion symmetry. In addition to explaining the theory of shift current, materials design opportunities and challenges will be discussed for future applications of the BPVE.
Introduction
The photovoltaic (PV) effect, which is the direct conversion of light to electricity, is regarded as one of the most reliable and abundant sources of renewable and clean energy. The power conversion efficiency (PCE, η) of a solar cell depends on a number of factors:
Here V_{oc} is the opencircuit voltage, J_{sc} is the shortcircuit current, FF is the fill factor and P_{in} is the power of the incident radiation on the solar cell. These quantities can be measured from the current–voltage (I–V) curve, as shown in Figure 1. In traditional solar cells, the mechanism for separation of the photoexcited carriers (electrons and holes) is the builtin electric field inside p–n junctions. Hot carriers typically relax to the bandedges via inelastic scattering events before being collected at the electrodes. These energy losses hamper the improvement of the PCE and limit the V_{oc} to the bandgap of lightabsorbing semiconductors. In addition, the requirement of p–n junctions for carrier separation demands careful interface engineering and sophisticated fabrication techniques.
In this review article, we discuss the bulk photovoltaic effect (BPVE), in particular, the shift current mechanism, which has a number of advantages over traditional p–n junctionbased solar cells. In the shift current mechanism, the driving force for carrier separation is not the builtin electric field, but the coherent evolution of electron and hole wavefunctions. Although the carriers in p–n junctions travel to the electrodes via driftdiffusive transport, shift current carriers instead rapidly propagate to the electrodes, minimising the opportunity for energy losses. Because this is a hot carrier effect, carrier separation does not depend on any internal electric fields (see the ‘Polarisation’ section), abovebandgap photovoltages can be generated, and the Shockley–Queisser limit could be surpassed. Because the shift current mechanism relies only on bulk inversion asymmetry, it can be realized in singlephase materials. The lack of p–n interface ensures that the entire PV material is active for current generation and allows for a simple and robust fabrication process.
In general, the symmetry requirement to produce a current from unpolarised light is to have a structure that allows for the definition of a unique spatial vector (i.e., a polar material). Therefore, materials with bulk inversion symmetry cannot generate photocurrents in the bulk. Materials that have broken bulk inversion symmetry but are nonpolar (e.g., GaAs) can generate bulk photocurrents, but only in response to polarised light.^{1} Ferroelectric materials, which have a switchable polarisation direction, satisfy the symmetry requirements for the generation of bulk photocurrents, and have historically been among the most studied BPVE materials.^{2–4} However, the switchable aspect is not a necessity for the observation of BPVE. In addition, we will show below (see the section ‘Polarisation’) that the BPVE response is not simply a measure of the strength of this polarisation field.
There are a number of BPVEs closely related to the shift current. Photocurrents can be generated in the bulk when scattering sites or absorption centres possess some amount of asymmetry.^{4–6} Such processes rely on the generation of an asymmetric distribution of nonthermalised carriers, in contrast to the coherent evolution in the shift current mechanism. These ballistic photocurrents have been discussed in ref. 7. In gyrotropic crystals, the switching of photocurrent directions with the helicity of circularly polarised light is known as the circular photogalvanic effect. In metals and semiconductors, under the assumptions of low frequencies and short relaxation times, this effect is controlled by the anomalous velocity that arises from orbital Berry phases.^{8–10} The circular photogalvanic effect has been experimentally observed in quantum wells.^{11–14} It has also been observed in tellurium crystals with significant spin–orbit valence band splittings.^{4,15}
The shift current BPVE has been observed in many materials systems, including ferroelectrics,^{2,3,16} quantum wells,^{17} organic crystals^{18} and twodimensional interfaces.^{19} The shift current theory was proposed as an explanation for the BPVE in BaTiO_{3} by von Baltz and Kraut,^{1} and was later derived within the framework of Green’s functions^{20} and nonlinear optics.^{21} Young and Rappe reformulated the shift current theory to enable efficient calculation from firstprinciples,^{22} and provided the first comparison of experimental BPVE data with shift current theory.^{22} In subsequent firstprinciples studies of the shift current in ferroelectric materials, it was shown that the shift current is the main contributor to the BPVE.^{23–30} As such, we will focus on the shift current.
In this review article, we provide an introduction to the basic theory and phenomenology of the shift current BPVE, with the aim of reviewing recent major developments in the field. In particular, there have been many recent efforts to increase shift current densities and efficiencies, and this will be the main focus of this review. We begin with a theoretical review of the shift current response, developed within the framework of a timedependent perturbation theory, in the section ‘Theory of the shift current response’. In the section ‘Material properties conducive to shift current response’, we will discuss intrinsic material properties conducive to shift current response with a tightbinding model. After a review of recent experimental studies of ferroelectric and polar materials for solar energy conversion in the section ‘Review of experiments’, we present firstprinciples studies of the shift current response in various real materials, with an emphasis on oxide and halide perovskites, in the section ‘Modern materials design for shift current’. The review concludes with a consideration of new directions for realising BPVEbased solar cells.
Theory of the shift current response
In the shift current mechanism, the behaviour of carriers immediately after excitation by light is governed by coherent excitation instead of inelastic scattering. The timedependent perturbation theory should therefore provide a good description of the electronic behaviour at these timescales. We first present a simplified derivation of the shift current in a threelevel system: the energy level n=0 is initially occupied, whereas the levels n=1 and n=2 are initially unoccupied. In the presence of an electric field E oscillating at frequency ω, the electron at n=0 evolves into a linear combination of n=0, 1 and 2. Within a firstorder timedependent perturbation theory, this state is
with the coefficients
Here V_{n0} and ω_{n0} are the dipole matrix element and energy difference between the levels n and 0. The current carried by the state ψ(t) is given by $J=\frac{e}{m}\u3008\psi (t)\leftP\right\psi (t)\u3009$, where P is the momentum operator and contains both oscillatory and constant components. The contribution to the constant current from the firstorder wavefunction is
where ${g}_{n\prime n}$ are phases derived from equation (3). The constant component of the current depends quadratically on the optical field and is a nonlinear optical effect. We note that the shift current also contains contributions from the momentum matrix elements between zeroth and secondorder wavefunctions in a timedependent perturbation theory (SMY and AMR, unpublished data).
Equations (2, 3, 4) describe the picture of electrons in a coherent, currentcarrying excited state ψ(t) that arises in an oscillating light field. Equivalently, these equations imply that an electron can be excited from the ground state 0 to a higher state n by a photon of frequency +ω, or it can be excited to a higher state $n\prime $ by a photon of frequency −ω. These two different excitation amplitudes interfere, giving a d.c. response, provided that the amplitudes interfere asymmetrically. That is, the matrix element describing the interference, ${V}_{n\prime 0}^{*}{V}_{n0}{P}_{n\prime n}$ in equation (4), does not vanish by symmetry. In real materials, this asymmetry is manifested in the different spatial character of conduction and valence bands.^{31} Heuristically, this causes the electrons (and holes) to ‘shift’ on excitation by light.
In general, the shift current J is related to the electric field via the frequency and materialdependent response function σ. In components:
Equation (5) shows that σ_{rsq} is a secondorder response function. The direction of the shift current is not necessarily the same as the applied electric field, as can be seen from the tensorial property of σ_{rsq}. The secondorder nature of the shift current response already imposes certain symmetry constraints on the classes of materials that can exhibit nonzero shift current response. In a material with inversion symmetry, the response function σ is left unchanged by an inversion operation, whereas the current and electric field, being vector quantities, each pick up a negative sign.
Using equation (6) in the constitutive equation (equation (5)) then implies that J_{q}=0 in such an inversion symmetric system. The shift current response can only be observed in materials with broken inversion symmetry. In the following sections, we will elaborate on the microscopic interpretation of this observation.
In crystalline materials, the response function can be written as an integral over the Brillouin zone.^{24}
where c and v are conduction and valence bands, respectively. The derivation of this integral is provided in ref. 21 using nonlinear susceptibilities and in ref. 20 using Green’s functions. Like linear absorption, the shift current response depends on the momentum matrix elements on a constant energy difference manifold given by ω_{c}−ω_{v}=ω. There is an additional factor R_{q}(c, v, k) that has dimensions of length and is known as the shift vector.^{20,21} In terms of the conduction and valence band wavefunction,
Here φ_{vc}(k) is the phase of the transition dipole$\u3008vk\left{P}_{r}\rightck\u3009$, and ${\chi}_{cq}(k)=\u3008{u}_{c}(k)\lefti\frac{\partial}{\partial {k}_{q}}\right{u}_{c}(k)\u3009$ is the Berry connection for band c, in terms of the Bloch functions u_{c}(k). Although each of the individual terms in equation (8) depends on the arbitrary gauge of the wavefunctions, their sum is gaugeindependent and is a welldefined physical quantity.^{22} Furthermore, by expressing the electric field in terms of the light intensity, the shift current response susceptibility can be shown to be proportional to light intensity. Although the shift current expression in equation (7) is appropriate for thin samples without significant attenuation of the incident light, corrections have to be made for bulk crystals where the light intensity is inhomogeneous. In the latter, where the light intensity is fully attenuated by the sample, the shift current is related to the incident light intensity by the Glass coefficient^{3}
where w is the width of the crystal surface exposed to illumination and α_{rr} is the absorption coefficient and I_{r} the light intensity along the direction of incident light polarisation. We will study both the shift current response function and the Glass coefficient in the following sections.
The PCE of the shift current mechanism we have described in this section is not the subject to the same limitations as ordinary photocurrent.^{32} As the shift current is generated by the incident illumination and does not depend on an external voltage, the photovoltage is not limited by the bandgap. In addition, the shift current is generally found to be insensitive to photovoltage, so that that total current is
where V is the photovoltage, J_{SC} is the shortcircuit shift current density, L is the distance between electrodes, and σ_{d} and σ_{ph} are the dark and photoconductivities, respecitively. Thus, the relationship between photovoltage and photocurrent is linear,^{33} implying a maximum fill factor of 0.25 (Figure 1a). The opencircuit photovoltage V_{OC} is then achieved when the shift current is fully cancelled by the backflow of conventional current that occurs due to thermalised carriers driven by the photovoltage. Thus, in the limit of a thin sample, and assuming that dark conductivity is negligible,
The maximum power that may be drawn is ${P}_{\mathrm{max}}=0.25{J}_{\mathrm{SC}}{V}_{\mathrm{OC}}{A}_{J}=0.25\frac{{{J}_{\mathrm{SC}}}^{2}L{A}_{J}}{{\sigma}_{\mathrm{ph}}}$ where A_{J} is the area through which J_{SC} flows. The total power absorbed by the sample is IA_{I}αd, where I is the intensity, A_{I} is the area illuminated, α is the absorption coefficient and d is the sample depth. The efficiency is then $\eta =0.25\frac{{{\sigma}_{\mathrm{SC}}}^{2}L{A}_{J}I}{{A}_{\mathrm{I}}\alpha d{\sigma}_{\mathrm{ph}}}$. At this point, we must recognise that there are at least two possible cell geometries. In the first, the electrode faces are normal to the illumination direction (Figure 1b), whereas in the second the electrode normal is perpendicular to the illumination direction (Figure 1c). In the former case, A_{I}=A_{J} and d=L, so that
If we assume that the photoconductivity is proportional to the number of carriers excited, then we may take it to be σ_{ph}=cμαI, where μ is the mobility, and we have
The same result may be obtained in the thinfilm limit for the second geometry. From this, it is clear that high efficiency requires maximising the Glass coefficient and minimising the mobility. The latter may be accomplished by creating heterostructures that feature regions with low mobility that the shift current is nonetheless able to flow through. An example of such a strategy was presented in ref. 34, where the authors show that domain walls of BFO possess very low photoconductivity, preventing carriers leaking back through the sample.
In this discussion of shift current efficiency, we have neglected the recombination current. In principle, geminate recombination of an electron–hole pair, which occurs before the electron and hole have separated, can result in a recombination current opposing the shift current, reducing the magnitude of the total photocurrent. However, in the usual setting of the BPVE, where the photocurrent arises primarily in the bulk of a strongly bonded material, the recombination current is likely to be negligible. This is because momentum scattering rates are many orders of magnitude faster than recombination rates in most semiconductors and insulators,^{20} and the momenta of electrons and holes are likely to be randomised before recombination occurs. In isolated or weakly bonded systems far from the bulk limit, this assumption may not apply. For instance, in an isolated polar diatomic molecule, only geminate recombination is present. However, as we show below (see the section ‘Delocalised electronic states’), we are often interested in the opposite limit of strongly delocalised electronic states, as these tend to give the largest shift current density. We note that momentum relaxation has the effect of homogeneous broadening; δfunctions are replaced by Lorentzians in equation (7), but the shift current magnitude is not expected to change.
Material properties conducive to shift current response
Polarisation
As we have seen above, the breaking of inversion symmetry is necessary for the shift current response. Materials with broken inversion symmetry can either be polar or nonpolar, and this has implications for the type of shift current response in these materials. As an example, consider the nonpolar noncentrosymmetric material hexagonal boron nitride (hBN). Unpolarised light with wavevector incident normal to the hBN plane does not break the threefold symmetry of the hBN lattice. In this situation, there is zero net shift current in the hBN plane.^{35} Therefore, to exhibit shift current under unpolarised light, polar noncentrosymmetric materials are required. Král has proposed removing the threefold symmetry of hBN by rolling a flat hBN sheet into a cylindrical nanotube.^{35} Such a structure can host a nonzero shift current in the presence of unpolarised light. Depending on the chirality of the nanotube, the shift current can have components along the length of the nanotube, as well as around the circumference of the nanotube. It is possible to study the relationship between the magnitude of the polarisation and the strength of the shift current response in this system by tuning the onsite potential difference between the boron and nitrogen sites in a tightbinding model. At small values of polarisation, the magnitude of the shift vector scales linearly with the polarisation, but the dependence becomes sublinear at higher values of polarisation.
The relationship between shift current response and polarisation is less straightforward in more complex materials. The shift current response of PbTiO_{3} was calculated using firstprinciples methods in ref. 22. The polarisation can be changed in the calculation by rigidly displacing the oxygen ions along a single Cartesian axis. The results reveal a complex relationship between the oxygen ion displacement and the shift current (Figure 2). At certain frequencies, an increase of the polarisation causes the shift current to first decrease in the magnitude and then reverse in the direction, whereas at other frequencies, the shift current response is relatively insensitive to the polarisation. Furthermore, a comparison with a related oxide perovskite BaTiO_{3} shows that despite PbTiO_{3} having more than twice the polarisation of BaTiO_{3}, both materials exhibit a similar shift current response.^{22} Therefore, although polarisation is necessary for the shift current response under unpolarised light, a larger polarisation does not always imply a larger shift current response. In equation (7), there is not an explicit dependence of the shift current on material polarisation. Rather, the correlations between shift current and material polarisation arise from how each depends on the breaking of inversion symmetry.
Bonding character
In addition to polarisation, the type of bonding in a system can also affect the magnitude of the shift current response. To understand these effects, we construct a simple onedimensional tightbinding model^{36} based on the Su–Shrieffer–Heeger model used in the study of conducting polymers.^{37} The tightbinding Hamiltonian is
This Hamiltonian describes a onedimensional chain of orbitals (Figure 3) with alternating onsite energies +Δ and −Δ. In addition, the bonds between the two inequivalent orbitals are alternating with strengths t+δ and t−δ. The parameter Δ controls the site asymmetry of the model, whereas the parameter δ controls the bonding character.
We have calculated the shift current response of this tightbinding model, and the results are displayed in Figure 3b. In the (δ, Δ) parameter space, the lines δ=0 and Δ=0 describe systems with no bond asymmetry and with no onsite energy asymmetry, respectively. The model has inversion symmetry in either of these cases, and the shift current vanishes at these lines. Away from these lines of high symmetry, a change in the sign of either Δ or δ changes the direction of the shift current. This is because changing the sign of Δ applies a bondcentred inversion operation to the system, while changing the sign of δ applies a sitecentred inversion operation. At a given value of Δ and δ, the direction of the shift current is dictated by the movement of electrons between sites A and B upon excitation. In ref. 38, explicit formulas are given for the bandedge shift current response of this onedimensional inversionbreaking model.
When t is set to 0, adjacent bonds have hopping integrals of different sign. In the context of the Slater–Koster tightbinding scheme, this can be interpreted as the orbitals A and B having different orbital characters. For example, if the A and B sites were s and p orbitals respectively, the spσ bonds between them would have hopping integrals of alternating sign. An increase in the magnitude of δ increases the magnitude of the shift current (Figure 3). This suggests that larger bond asymmetries tend to result in higher shift current responses. On the other hand, the site asymmetry parameter Δ is not well correlated with the shift current magnitude (Figure 3b). This is consistent with the general observation made in the previous section that there does not seem to be a simple relationship between polarisation and shift current.
Delocalised electronic states
In this section, and in ref. 36 (SMY and AMR, unpublished data), the tightbinding model of the section ‘Bonding character’ is extended by introducing hopping beyond nearest neighbours. We let the higherorder hopping amplitudes decay exponentially with distance by parameterising them as ${e}^{{R}_{l}/\xi}$, with ξ>0 and R_{l} a lattice vector. We have found that the magnitude of the shift vector is enhanced significantly by the presence of higherorder hopping, particularly near the Γ point of the Brillouin zone (Figure 4). As the higherorder hopping increases, the bandwidth and band dispersion increase also, particularly at the Γ point. As the wavefunctions therefore become more delocalised with higherorder hopping, this implies a correlation between delocalised electronic states and large shift current. Away from Γ, the wavefunctions pick up a phase that varies rapidly in space, resulting in destructive interference and diminishing the effects of higherorder hopping.
These observations are supported by our density functional theory (DFT) calculation of shift current in PbTiO_{3}.^{22} We find that large shift current occurs when the states involved in the transition have a strong bonding or antibonding character along the Ti–O chains collinear with the direction of polarisation. On the other hand, nonbonding states, such as those comprising only oxygen or titanium orbitals, have a weaker shift current response. Heuristically, currentcarrying excited states are more likely to be constructed from a superposition of delocalised orbitals rather than heavily localised orbitals.
We have therefore identified two factors that contribute to large shift current response. Promising candidate materials are those with strong covalent bonds that imply highly delocalised states. Wavefunction asymmetry, due either to large atomic displacements from highsymmetry structures or to atomic species with varied orbital characters, will generally increase the shift current response.
Review of experiments
The BPVE in ferroelectric materials has been explored experimentally for >50 years. In many of the older papers on BPVE (e.g., refs 39–41), the measured photocurrents were given different names (optical damage, anomalous PV effect, photogalvanic effect, abovebandgap optical rectification and resonant nonlinear susceptibility), and were only reinterpreted as the shift current^{42} and referred to as such after the development of the shift current theory. In ferroelectrics, the application of an external electric field is not necessary for the generation of photocurrent, as demonstrated in early work on the prototypical ferroelectric BaTiO_{3},^{43} where the photocurrent was attributed to surface spacecharge layers. This was followed by studies^{3,44–47} showing the presence of photocurrents and photovoltages in many other ferroelectrics. The authors of refs 3,47 were the first to propose that the generation of photocarriers in the bulk of a ferroelectric was the direct consequence of the unique axis of polarisation. Further developments include the strong dependence of photocurrent on light polarisation direction in BaTiO_{3},^{39} and a giant BPVE in LiNbO_{3} (ref. 48) scaling linearly with light intensity.
Following the development of the shift current theory,^{1,21,35} there appeared experiments that discussed the shift current, and in particular, its relation to other nonlinear optical effects. Abovebandgap optical rectification, which was later understood to be dominated by the shift current,^{42} was measured in GaAs^{40} and modelled from the perspective of the nonlinear optical susceptibility.^{41} Experiments on semiconductor quantum wells have distinguished between shift currents and circular photogalvanic currents.^{49,50} An estimate of the shift vector was extracted by comparing a phenomenological model for shift currents with the experiments on wurtzite semiconductors,^{51} while a shift current model was used to understand the ultrafast optical response of GaAs.^{52} In ferroelectrics, a direct comparison of ab initio shift current calculations with experiment has provided support for the shift current theory.^{22,53} Recently, shift current effects have been studied in the highfield, lowfrequency regime,^{16} whereas the effect of Coulombic interactions on the shift current have also been studied experimentally.^{17}
Shift currents have also been measured in systems other than bulk ferroelectrics, such as GaAs quantum wells and surfaces. Due to the T_{d} symmetry of GaAs, only xyz, zxy, yzx, yxz, zyx and yzx tensor elements are nonzero. Bieler et al.^{17,54} reported additional nonzero tensor elements of the shift current in semiconductor quantum wells because of symmetry reduction of the quantum well structure. Furthermore, this quantum confinementinduced BPVE is also observed recently in ferroelectric heterojunctions. Nakamura et al.^{19} have measured the photocurrent in LaFeO_{3}/SrTiO_{3} heterojunctions with varying LaFeO_{3} thickness. This work illustrates the coexistence of the shift current and the drift current (induced by internal electric field) with opposite directions. By manipulating the LaFeO_{3} layer thickness, the polarisation magnitude can be changed, introducing sign change of the total photocurrent due to the competing contributions of the shift current and the drift current. With the decrease of the system dimensions, the BPVE is also observed in onedimensional molecules and organic crystals. Ogden and Gookin^{18} measured the BPVE in a prototypical organic polymer with net electric dipole moment >30 years ago. Recently, Vijayaraghavan et al.^{55} observed the BPVE of 1,4diphenylbutadiene crystal with πconjugated molecules, providing experimental evidence for the BPVE in polar organic crystals.
It was found that BPVE is enhanced in nanostructures.^{56} For example, (Pb,La)(Zr,Ti)O_{3} (PLZT) and its solid solutions in a thinfilm form can have high photocurrent magnitude. Ichiki et al.^{57} observed higher BPVE in a crystallographically oriented PZT film than in a randomly oriented film. Qin et al.^{58} reported that decreasing film thickness is an effective way to engineer BPVE and increase the efficiency markedly, which is further supported by the giant BPVE observed in BaTiO_{3} thin films.^{56} Pintilie et al. have measured the shortcircuit photocurrent of Pb(Zr,Ti)O_{3} (PZT) polycrystalline layers and epitaxial films under different light frequencies. The direction of the photocurrent flips when the polarisation of the film is reversed by applying voltage.^{59,60}
Materials with low bandgaps and high polarisations have attracted considerable attention in PV material design. There have been many studies on understanding and optimising the BPVE in BiFeO_{3} (BFO)^{34,61–65}, because of its relatively low bandgap (2.3–2.8 eV), high polarisation (90 μC/cm^{2})^{66} and functional optical properties.^{67} In particular, the observed large opencircuit voltage^{34,61,62} suggests its use as a potential PV material. Choi et al.^{68} reported a diodelike effect in a singledomain BFO crystal, and the direction of the diode is determined by the polarisation of the crystal and can be switched by larger external fields. This ability to switch the BPVE direction in BFO is also supported by measurements of Ji et al.^{69} on an epitaxial BFO thin film. The photocurrent was observed to flow in the opposite direction of the BFO polarisation, and the current is switchable by switching the polarisation direction. Recently, [KNbO_{3}]_{1−x} [BaNi_{1/2}Nb_{1/2}O_{3−δ}]_{x} (KBNNO) with large bandgap tunability (E_{g}=1.1–3.8 eV) and spontaneous polarisation was found to generate BPVE photocurrent ~50 times larger than that of the ferroelectric PLZT, suggesting potential applications in PV solar cells.^{70}
As mentioned above, the excellent PV properties of BFO are likely related to its large polarisation and low bandgap compared with other ferroelectrics. However, there are many other factors that affect the BPVE in BFO. Seidel et al.^{62} observed that domain walls have a critical role in carrier generation and recombination. Including more domain walls gives rise to higher opencircuit photovoltage^{61} and enhances the photoconductivity of BFO.^{35} On the other hand, Alexe et al.^{71} suggested that shallow defect levels in the bandgap of BFO are important. Interestingly, in ref. 69, nonzero BPVE was observed in singledomain BFO perpendicular to the polarisation direction, showing that for various space groups, BPVE need not be along the ferroelectric polarisation direction.^{68,72,73}
The role of defects in the BPVE is also emphasised, showing that oxygen vacancies are important for the electricfieldinduced switching PV diode effect^{74,75} and the photoconductivity.^{76–78} Furthermore, the BPVE and photorefractive effect in irondoped LiNbO_{3} have been studied for a long time,^{79–83} demonstrating the significant role of Fe in enhancing the performance. The photorefractive effect, or ‘optical damage’, is caused by the BPVE without electrodes, leading to a spacecharge field that changes the refractive index via the electrooptic effect.^{80} Recently, Crdoped BFO (including BFO and BiCrO_{3} solid solutions) has attracted great interest. Nechache et al.^{84} have observed 6% PCE in Bi_{2}FeCrO_{6} epitaxial thin films. Moreover, this material shows strong bandgap tunability (as high as 1 eV) by varying the Bsite cation ordering and ordered domain size, and ≈8% PCE was reported in a multilayer configuration of this material.^{85} In these complex materials with dopants and defects, inelastic scattering may have a role in PV response, and other theories besides the shift current may be necessary in these cases.^{7}
Modern materials design for shift current
In this section, we apply shift current design principles to a wide variety of real materials, and study their shift current responses, calculated within the firstprinciples formalism introduced in the section ‘Theory of the shift current response’.
Polar order engineering
The starting point of shift current materials design is the breaking of inversion symmetry, which is essential for the shift current response. The ferroelectric oxides, with their switchable polar order, are a natural class of materials to consider.
First, we consider the wellknown room temperature multiferroic material BFO. In the following, the polarisation direction is taken to be the z direction. The R3c space group of BFO only allows a few nonzero tensor elements for its BPVE responses, which can be computed from first principles using the shift current theory outlined in the section ‘Theory of the shift current response’. To calculate the shift current response, the electronic structure of BFO must first be computed. Young et al. used the DFT+U method along with a semicore pseudopotential for Fe to improve the description of the 3d electrons and correctly describe the antiferromagnetic physics in this material, giving E_{g}=2.58 eV. Shown in Figure 5c,b are the yyY components of the Glass coefficient and shift current response tensor σ as a function of light frequency.^{24} The response occurs at photon energies higher than the bandgap of the bulk. As shown in the spectra, the experimentally measured shift current and Glass coefficient perpendicular to the polarisation^{63} are in good agreement with calculations. Current in directions perpendicular to the polarisation should not contain contributions directly generated by the polarisation, such as the depolarisation field photocurrent. Therefore, these results establish that the shift current mechanism has a significant role in the BPVE of BFO.
Besides explaining the BPVE in BFO, the firstprinciples approach to computing shift current has also successfully explained the BPVE in the prototypical ferroelectrics BaTiO_{3} (BTO) and PbTiO_{3} (PTO), and provides further guidelines for designing materials with large BPVE. Shown in Figure 6 is the comparison between experimentally measured I(ω)^{39} and computed shift current response spectrum for BTO.^{22} The shaded region indicates the experimental error bars using parameters from the original experiment. The calculated shortcircuit photocurrents agree with the measurements very well in terms of both direction and magnitude.
Although materials that are almost nonpolar tend to have small shift current responses (see the discussion of hybrid perovskites in the section ‘Wavefunction engineering’), a larger polarisation does not always lead to larger shift currents. To understand the relationship of shift vector and shift current to polarisation, these quantities are calculated while manually moving the atoms to vary the polarisation magnitude. As illustrated in Figure 2a, the dependence of shift vectors on polarisation can be nonlinear. Even the direction of the shift current may not be related to the direction of the bulk polarisation, and the current direction can change as a function of light frequency (Figure 6).
These observations suggest that the material polarisation does not determine the shift current magnitude and direction. Instead, there are other factors related to the electronic structure of the materials which strongly affect shift current magnitudes. These will be analysed in the following sections.
Electronic structure engineering
In this section, we examine electronic structure design principles for high shift current responses: (1) engineering delocalised orbital characters using s and p orbitals; (2) the need for an appropriate bandgap in the visible light region; (3) attaining high density of states using materials with lowdimensional components.
Wavefunction engineering
The tightbinding results of the section ‘Delocalised electronic states’ suggest that delocalised electronic states are beneficial for large shift currents, as they are more likely to support currentcarrying excited states. In PTO, DFT calculations^{22} show that states with delocalised character tend to give high shift current responses (Figure 2b), whereas nonbonding or strongly localised states tend to give low shift current. Transitions involving bands with strong contributions from transition metals with localised d orbitals tend to have small shift vectors.
A family of materials with strong s and p orbital characters in the valence and conduction bands is the organometalhalide perovskites (OMHPs). They have attracted huge interest due to their rapidly increasing PCE. Appropriate bandgaps within the visible light range,^{86} long carrier lifetime,^{87} and strong light absorption^{88} make these materials promising for PV solar cells. To illustrate the above ideas about wavefunction delocalisation, we consider the most studied OMHP—CH_{3}NH_{3}PbI_{3} (MAPbI_{3}), which has a dipolar molecular cation at each Asite.^{89} We consider configurations of MAPbI_{3} that break inversion symmetry and thereby allow BPVE.
The valence bands MAPbI_{3} are primarily of Pb 6s and I 5p characters,^{90} which is reminiscent of the simplified tightbinding model introduced in the section ‘Bonding character’. The shift current response in MAPbI_{3} has been computed,^{27} including spin–orbit coupling,^{90–92} in two types of structures: one with all the molecular dipole moments aligned (M1) and another in which all the molecular dipole moments nearly cancel with neighboruing molecules (M2). The nearly nonpolar M2 structure has a much smaller shift current response than M1 (Figure 7). The importance of the strongly delocalised states involved in the phototransitions in MAPbI_{3} is demonstrated by the fact that MAPbI_{3} has a shift current magnitude comparable to that of BFO, despite having a much smaller polarisation (≈5 μC/cm^{2} in the z direction) than BFO (≈100 μC/cm^{2}).
The delocalised nature of the conduction and valance band states in MAPbI_{3} can be further increased by Cl doping. It was shown that doping Cl at the equatorial positions increases the shift current of the M1 structure, giving an approximately three times larger shift current response than BFO. The equatorial Cl doping results in structural distortions and hybridisation of the conduction band Pb 6p_{x/y} orbitals with the halide p orbitals, leaving the Pb 6p_{z} orbitals as the dominant orbital character of the conduction band. As p_{z} is more delocalised in the direction of current (z) than p_{x/y}, this results in an enhanced shift current. Experimentally, Cl doping enhances the ordinary PV effect in MAPbI_{3} greatly, although the origin of this effect is still under debate.^{93–95}
Another materials design strategy in the OMHPs is the substitution of A and Bsite members of the perovskite structure. By introducing Ge on the Bsite and having both Cs and organic molecules as Asite in OMHPs, the resulting materials show spontaneous polarisation as a consequence of the Ge^{2+} lone pair, and they exhibit large secondharmonic generation.^{96} Such a strategy might also hold promise for the shift current response, which, like secondharmonic generation, is a nonlinear optical effect.
Bandgap engineering
It is desirable for the bandgap of a shift current material to lie in the visible spectrum, if it is to be used in solar power lightharvesting devices. In this section, we focus on ways to control the onset of light absorption and shift current generation, using the recently synthesised low bandgap ferroelectric material (K,Ba)(Ni,Nb)O_{3−δ} (KBNNO)^{70,97,98} as an example.
One method of controlling the bandgap is by introducing sitespecific aliovalent substitutions^{99} and vacancies into the parent material KNbO_{3}.^{100,101} Oxygen vacancies may have both positive and negative effects on the functional properties of materials. For example, oxygen vacancies are one of the most important providers of ntype carriers, making them beneficial for ntype semiconductors, but O vacancies remove ptype carriers, making them detrimental for ptype semiconductors. For PV and photocatalytic materials, oxygen vacancies are generally detrimental, because they can enhance the charge recombination rate and reduce the mean free path of the charge carriers. Nevertheless, oxygen vacancies can also be incorporated purposefully to reduce conventional mobility (which enhances V_{oc}, equation (1)), to compensate charge, and to induce desired structural changes, as we show here in KBNNO.
In this material, the substitutional defects involve Ni^{2+} ions replacing Nb^{5+} ions, Ba^{2+} ions replacing K^{+} ions and charge compensation by O vacancies. We consider two structural configurations of (2/3)KNbO_{3}(1/3)Ba(Ni_{1/2}Nb_{1/2})O_{11/4} with two Ni^{2+} substitutions each. In one configuration (C_{1} configuration), the two Ni ions are distributed along the body diagonal direction with the O vacancy adjacent to only one Ni^{2+} ion (NiO_{6} and NiO_{5}), whereas in the other (C_{2} configuration), the two Ni ions are aligned along the Cartesian z axis with one O vacancy in between, leaving both Ni^{2+} an environment of O_{5} (two NiO_{5}).
Compared with the C_{2} configuration, the C_{1} configuration exhibits a larger Glass coefficient and a lower onset photon energy (Figure 8). These two arrangements have very different electronic structure properties. In the C_{1} arrangement, Nb and Ni orbitaldominated gap states are induced, leading to a smaller bandgap. In the C_{2} arrangement, these states move deeper into the valence band, and O 2p orbitals dominate the top of the valence band. This difference in the electronic properties is ascribed to their different structural properties. The larger lattice asymmetry corresponding to the NiO_{5} complex induces a much bigger splitting between the ${d}_{{z}^{2}}$ and ${d}_{{x}^{2}{y}^{2}}$ orbitals and a much lower energy of the ${d}_{{z}^{2}}$ orbital than those for the NiO_{6} complex. As a result, gap states are induced for the C_{1} arrangement because it also contains NiO_{6} complexes, but in the C_{2} arrangement these states do not contribute to the bandedge electronic transitions, as only NiO_{5} complexes are involved. Therefore, by moving O vacancies away from Ni, the shift current is significantly enhanced and this effect is accomplished through the change of structural and electronic orbital character properties.
Strain is another method of controlling the bandgap. It is widely applied via epitaxial growth of thin films in order to achieve desired functional properties, as it can substantially affect the octahedral cage distortions, rotate the polarisation and change the electronic structure of perovskites.^{102–104} We consider applying inplane compressive strain to the (2/3)KNbO_{3}(1/3)Ba(Ni_{1/2}Nb_{1/2})O_{11/4} solid solution. The configuration we adopt here includes two Ni atoms at the body diagonal positions (C_{1}). Our results show that compressive strains increase the shift current onset photon energy (Figure 8). A detailed electronic structure and wavefunction analysis indicates that the applied compressive strains drive the original ${d}_{{z}^{2}}$ orbitaldominated gap states to shift downwards in energy and finally merge into the valence band.^{28} This gives rise to a larger band gap and also reduces the magnitude of the shift current response. To make use of the beneficial effect of inplane compressive strains, materials must have delocalised electronic orbitals that can be shifted to bandedges by these strains.
Apart from defects and strain, other methods are available for tuning the properties of KBNNO. Recently, manipulation of local polar order (potential gradients) has been proposed as a way to control shift current response in solid solutions in this material.^{30}
Density of states engineering
Another approach for increasing shift currents is designing materials with large density of states near the bandedges.^{38} The shift current responses at frequencies close to the bandgap energy are often the most relevant for large bandgap semiconductors, as they fall in the visible light spectrum. Furthermore, firstprinciples calculations show that the shift vector is often large near the bandgap. Onedimensional structures have increased joint densities of states near the bandgap energy, magnifying the shift current at this energy. This suggests that lowdimensional materials such as chain and layerlike structures may be promising materials with large BPVE.
The alkalimetal chalcogenides are a class of materials with this property. Many members of the class, such as KPSe_{6}, K_{2}P_{2}Se_{6}, LiAsSe_{2}, LiAsS_{2} and NaAsSe_{2} show bandgaps in visible light region.^{105} It was also found that some of them show spontaneous polarisation and strong secondharmonic generation responses.^{105,106} We consider the shift current responses of LiAsSe_{2}, LiAsS_{2} and NaAsSe_{2}. All three materials have been synthesised in polar monoclinic space group, with Cc for LiAsSe_{2} and LiAsS_{2}, and Pc for NaAsSe_{2}. Figure 9 shows that these three compounds have onedimensional AsX chain (X=Se, S) motifs. The orbitals of the states near the bandgap are mainly s and p orbitals coming from P, As or Se, with a strong covalent character.
Shown in Figure 9 is the shift current response spectrum of LiAsSe_{2}, with the dashed line indicating the shift current response of BFO (with a magnitude of σ≈3×10^{−4} (A/m^{2})/(W/m^{2})). Due to the wellknown issue of underestimation of band gaps in DFT, the LiAsSe_{2} spectrum has been shifted to have the experimental bandgap (1.11 eV).^{24} The zzZ component of LiAsSe_{2} shift current shows broad and high magnitude, displaying around 50 times larger response than BFO, making it a potential candidate for solar cell materials. LiAsS_{2} shows similar spectrum line shape to LiAsSe_{2} but with smaller magnitude. This may be because the bonds between As and S are not as covalent as between As and Se. These results for the alkalimetal chalcogenides suggest that materials with a strong degree of anisotropy and onedimensional conducting channels can potentially have large shift current responses.
Conclusions and outlook
In this review, we have examined the factors contributing to the shift current response arising from exciting a currentcarrying coherent state. The breaking of inversion symmetry is necessary, but there are many other electronic structure factors affecting the shift current magnitude. We have seen that it is desirable to have a bandgap in the visible spectrum, as well as a large density of states at the bandedges to efficiently capture incident light. Once excited, the shift current carriers rapidly propagate to the electrodes via coherent evolution of the currentcarrying state. For this purpose, it is beneficial to have highly delocalised conduction or valence band states, to aid in the coherent evolution of the carriers from the bulk of the material to the electrodes. There are many specific materials design approaches that can be used to achieve these requirements, such as substitutional doping, the introduction of vacancies, the application of strain and the use of lowdimensional materials. In addition, it has recently been suggested that the tuning of topological phase transitions^{29} can enhance the shift current response.
A remaining open question is the calculation of the PCE of a shift current material. The formalism developed in the section ‘Theory of the shift current response’ is useful for calculating the shortcircuit current, but the opencircuit voltage, one of the important factors contributing to the PCE, is less amenable to calculation using periodic boundary conditions. Furthermore, the opencircuit voltage depends on factors external to the shift current theory, such as the total conductivity, which is not generally a bulk quantity. A related issue is the effect of electrodes on the measured photocurrent. Careful selection of electrode materials has improved PCE in the linear response regime, and it is likely that a similar effect exists for shift current materials. The study of the temporal shift current response beyond the continuous wave limit,^{53,107} the topological aspects of nonlinear optics^{29,108} and the effect of excitons^{109} have also become interesting directions of research in recent years. It is expected that shift current is preserved in the presence of excitons.^{109}
In summary, the nascent applications of polar materials in PV applications call for a clear understanding of the origin of the BVPE. Understanding and quantifying the interplay between bulk photocurrent, material compositions, nanostructures, strains and structural defects will help to realise the true potential of BVPE. Distinguishing the truly bulk effect from the interfacial effect in ferroelectrics will inspire device engineering guidelines to apply both mechanisms for solar energy conversion. The shift current theory provides a valuable tool to discover, design and optimise materials for BVPEbased devices with firstprinciples methods. We believe that with concerted experimental and theoretical efforts, the BVPE will find its applications in the PV industry.
References
 1
von Baltz, R. & Kraut, W. Theory of the bulk photovoltaic effect in pure crystals. Phys. Rev. B 23, 5590–5596 (1981).
 2
Auston, D. H., Glass, A. M. & Ballman, A. A. Optical rectification by impurities in polar crystals. Phys. Rev. Lett. 28, 897–900 (1972).
 3
Glass, A. M., von der Linde, D. & Negran, T. J. Highvoltage bulk photovoltaic effect and photorefractive process In LiNbO3 . Appl. Phys. Lett. 25, 233–235 (1974).
 4
Fridkin, V. M. Bulk photovoltaic effect in noncentrosymmetric crystals. Crystallogr. Rep. 46, 654–658 (2001).
 5
Belinicher, V. I. & Sturman, B. I. The photogalvanic effect in media lacking a center of symmetry. Sov. Phys. Usp. 23, 199 (1980).
 6
Butler, K. T., Frost, J. M. & Walsh, A. Ferroelectric materials for solar energy conversion: photoferroics revisited. Energy Environ. Sci. 8, 838–848 (2015).
 7
Belinicher, V. I. The relation between shift and ballistic currents in the theory of photogalvanic effect. Ferroelectrics 83, 29–34 (1988).
 8
Deyo, E., Golub, L. E., Ivchenko, E. L. & Spivak, B. Semiclassical theory of the photogalvanic effect in noncentrosymmetric systems. Preprint at https://arxiv.org/abs/0904.1917 (2009).
 9
Moore, J. E. & Orenstein, J. Confinementinduced berry phase and helicitydependent photocurrents. Phys. Rev. Lett. 105, 026805 (2010).
 10
Sodemann, I. & Fu, L. Quantum nonlinear hall effect induced by berry curvature dipole in timereversal invariant materials. Phys. Rev. Lett. 115, 216806 (2015).
 11
Ganichev, S. D. et al. Conversion of spin into directed electric current in quantum wells. Phys. Rev. Lett. 86, 4358–4361 (2001).
 12
Diehl, H. et al. Spin photocurrents in (110)grown quantum well structures. N. J. Phys. 9, 349 (2007).
 13
Olbrich, P. et al. Observation of the orbital circular photogalvanic effect. Phys. Rev. B 79, 121302 (2009).
 14
Karch, J. et al. Photoexcitation of valleyorbit currents in (111)oriented silicon metaloxidesemiconductor fieldeffect transistors. Phys. Rev. B 83, 121312 (2011).
 15
Sturman, B. I. & Fridkin, V. M. The Photovoltaic and Photorefractive Effects in Noncentrosymmetric Materials 8 (Breach Science Publishers, 1992).
 16
Somma, C., Reimann, K., Flytzanis, C., Elsaesser, T. & Woerner, M. Highfield terahertz bulk photovoltaic effect in lithium niobate. Phys. Rev. Lett. 112, 146602 (2014).
 17
Bieler, M., Pierz, K., Siegner, U. & Dawson, P. Shift currents from symmetry reduction and Coulomb effects in (110)orientated GaAs∕Al0.3Ga0.7As quantum wells. Phys. Rev. B 76, 161304 (2007).
 18
Ogden, T. R. & Gookin, D. M. Bulk photovoltaic effect in polyvinylidene fluoride. Appl. Phys. Lett. 45, 995–997 (1984).
 19
Nakamura, M. et al. Spontaneous polarization and bulk photovoltaic effect driven by polar discontinuity in LaFeO3/SrTiO3 heterojunctions. Phys. Rev. Lett. 116, 156801 (2016).
 20
Král, P. Quantum kinetic theory of shiftcurrent electron pumping in semiconductors. J. Phys. Condens. Matter 12, 4851 (2000).
 21
Sipe, J. E. & Shkrebtii, A. I. Secondorder optical response in semiconductors. Phys. Rev. B 61, 5337–5352 (2000).
 22
Young, S. M. & Rappe, A. M. First principles calculation of the shift current photovoltaic effect in ferroelectrics. Phys. Rev. Lett. 109, 116601 (2012).
 23
Nastos, F. & Sipe, J. E. Optical rectification and current injection in unbiased semiconductors. Phys. Rev. B 82, 235204 (2010).
 24
Young, S. M., Zheng, F. & Rappe, A. M. Firstprinciples calculation of the bulk photovoltaic effect in bismuth ferrite. Phys. Rev. Lett. 109, 236601 (2012).
 25
Young, S. M., Zheng, F. & Rappe, A. M. Prediction of a linear spin bulk photovoltaic effect in antiferromagnets. Phys. Rev. Lett. 110, 057201–057201 (2013).
 26
Brehm, J. A., Young, S. M., Zheng, F. & Rappe, A. M. Firstprinciples calculation of the bulk photovoltaic effect in the polar compounds LiAsS2, LiAsSe2, and NaAsSe2 . J. Chem. Phys. 141, 204704 (2014).
 27
Zheng, F., Takenaka, H., Wang, F., Koocher, N. Z. & Rappe, A. M. Firstprinciples calculation of the bulk photovoltaic effect in CH3NH3PbI3 and CH3NH3PbI3xClx . J. Phys. Chem. Lett. 6, 31–37 (2015).
 28
Wang, F. & Rappe, A. M. Firstprinciples calculation of the bulk photovoltaic effect in kNbO3 and (K,Ba)(Ni,Nb)O3δ . Phys. Rev. B 91, 165124 (2015).
 29
Tan, L. Z. & Rappe, A. M. Enhancement of the bulk photovoltaic effect in topological insulators. Phys. Rev. Lett. 116, 237402 (2016).
 30
Wang, F., Young, S. M., Zheng, F., Grinberg, I. & Rappe, A. M. Substantial bulk photovoltaic effect enhancement via nanolayering. Nat. Commun. 7, 10419 (2016).
 31
Nastos, F. & Sipe, J. E. Optical rectification and shift currents in GaAs and GaP response: Below and above the band gap. Phys. Rev. B 74, 035201 (2006).
 32
Shockley, W. & Queisser, H. J. Detailed balance limit of efficiency of pn junction solar cells. J. Appl. Phys. 32, 510–519 (1961).
 33
Gunter, P. & Micheron, F. Photorefractive effects and photocurrents in KNbO3: Fe. Ferroelectrics 18, 27–38 (1978).
 34
Bhatnagar, A., Roy Chaudhuri, A., Heon Kim, Y., Hesse, D. & Alexe, M. Role of domain walls in the abnormal photovoltaic effect in BiFeO3 . Nat. Commun. 4, 28351–28358 (2013).
 35
Král, P., Mele, E. J. & Tománek, D. Photogalvanic Effects in Heteropolar Nanotubes. Phys. Rev. Lett. 85, 1512–1515 (2000).
 36
Young, S. M. Theory of the Bulk Photovoltaic Effect in Oxides, and FirstPrinciples Computational Design of Materials with Bulk Dirac Points. PhD Dissertation, 1–220 (University of Pennsylvania ScholarlyCommons, 2011).
 37
Su, W. P., Schrieffer, J. R. & Heeger, A. J. Solitons in polyacetylene. Phys. Rev. Lett. 42, 1698–1701 (1979).
 38
Cook, A. M., Fregoso, B. M., Juan, F. & de Moore, J. E. Design principles for shift current photovoltaics. Preprint at http://arxiv.org/abs/1507.08677 (2015).
 39
Koch, W. T. H., Munser, R., Ruppel, W. & Wurfel, P. Anomalous Photovoltage In Batio3. Ferroelectrics 13, 305–307 (1976).
 40
Zhang, X.C., Jin, Y., Yang, K. & Schowalter, L. J. Resonant nonlinear susceptibility near the GaAs band gap. Phys. Rev. Lett. 69, 2303–2306 (1992).
 41
Chuang, S. L., SchmittRink, S., Greene, B. I., Saeta, P. N. & Levi, A. F. J. Optical rectification at semiconductor surfaces. Phys. Rev. Lett. 68, 102–105 (1992).
 42
Côté, D., Laman, N. & van Driel, H. M. Rectification and shift currents in GaAs. Appl. Phys. Lett. 80, 905–907 (2002).
 43
Chynoweth, A. G. Surface spacecharge layers in barium titanate. Phys. Rev. 102, 705–714 (1956).
 44
Chen, F. S. Optically induced change of refractive indices in LiNbO3 and LiTaO3 . J. Appl. Phys. 40, 3389–3396 (1969).
 45
Grekov, A. A., Malitskaya, M. A., Spitsnya, V. D. & Fridkin, V. M. Photoferroelectric effects in ferroelectric semiconductors of the A^{V}B^{VI}C^{VII} type with lowtemperature phase changes. Sov. Phys. Crystallogr. 15, 500 (1970).
 46
Fridkin, V., Grekov, A., Ionov, P., Rodin, A., Savchenko, E. & Mikhailina, K. Photoconductivity in certain ferroelectrics. Ferroelectrics 8, 433–435 (1974).
 47
Glass, A. M., Linde, D., von der Auston, D. H. & Negran, T. J. Excited state polarization, bulk photovoltaic effect and the photorefractive effect in electrically polarized media. J. Electron. Mater. 4, 915–943 (1975).
 48
Dalba, G., Soldo, Y., Rocca, F., Fridkin, V. M. & Sainctavit, P. Giant bulk photovoltaic effect under linearly polarized xray synchrotronradiation. Phys. Rev. Lett. 74, 988–991 (1995).
 49
Ganichev, S. D. et al. Removal of spin degeneracy in pSiGe quantum wells demonstrated by spin photocurrents. Phys. Rev. B 66, 075328 (2002).
 50
Bieler, M., Pierz, K. & Siegner, U. Simultaneous generation of shift and injection currents in (110)grown GaAs/AlGaAs quantum wells. J. Appl. Phys. 100, 083710 (2006).
 51
Laman, N., Bieler, M. & van Driel, H. M. Ultrafast shift and injection currents observed in wurtzite semiconductors via emitted terahertz radiation. J. Appl. Phys. 98, 103507 (2005).
 52
Kohli, K. K., Mertens, J., Bieler, M. & Chatterjee, S. Pulseshaperassisted coherent control of shift currents. J. Opt. Soc. Am. B 28, 470–474 (2011).
 53
Daranciang, D. et al. Ultrafast photovoltaic response in ferroelectric nanolayers. Phys. Rev. Lett. 108, 08760116 (2012).
 54
Bieler, M., Laman, N., van Driel, H. M. & Smirl, A. L. Ultrafast spinpolarized electrical currents injected in a strained zinc blende semiconductor by single color pulses. Appl. Phys. Lett. 86, 061102 (2005).
 55
Vijayaraghavan, R. K. et al. Bulk photovoltaic effect in an organic polar crystal. Chem. Commun. 50, 6530–6533 (2014).
 56
Zenkevich, A., Matveyev, Y., Maksimova, K., Gaynutdinov, R., Tolstikhina, A. & Fridkin, V. Giant bulk photovoltaic effect in thin ferroelectric BaTiO3 films. Phys. Rev. B 90, 161409 (2014).
 57
Ichiki, M. et al. Photovoltaic properties of (Pb,La)(Zr,Ti)O3 films with different crystallographic orientations. Appl. Phys. Lett. 87, 222903–1–3 (2005).
 58
Qin, M., Yao, K. & Liang, Y. C. High efficient photovoltaics in nanoscaled ferroelectric thin films. Appl. Phys. Lett. 93, 122904–1–3 (2008).
 59
Pintilie, L., Vrejoiu, I., Le Rhun, G. & Alexe, M. Shortcircuit photocurrent in epitaxial lead zirconatetitanate thin films. J. Appl. Phys. 101, 064109–1–8 (2007).
 60
Pintilie, L., Stancu, V., Vasile, E. & Pintilie, I. About the complex relation between shortcircuit photocurrent, imprint and polarization in ferroelectric thin films. J. Appl. Phys. 107, 114111 (2010).
 61
Yang, S. et al. Abovebandgap voltages from ferreoelectric photovoltaic devices. Nat. Nano 5, 143–147 (2010).
 62
Seidel, J. et al. Efficient Photovoltaic Current Generation at Ferroelectric Domain Walls. Phys. Rev. Lett. 107, 126805 (2011).
 63
Ji, W., Yao, K. & Liang, Y. C. Evidence of bulk photovoltaic effect and large tensor coefficient in ferroelectric BiFeO3 thin films. Phys. Rev. B 84, 094115 (2011).
 64
Alexe, M. & Hesse, D. Tipenhanced photovoltaic effects in bismuth ferrite. Nat. Commun. 2, 256 (2011).
 65
Yang, S. Y. et al. Photovoltaic effects in BiFeO3 . Appl. Phys. Lett. 95, 062909–1–3 (2009).
 66
Catalan, G. & Scott, J. F. Physics and applications of bismuth ferrite. Adv. Mater. 21, 2463–2485 (2009).
 67
Kundys, B., Viret, M., Colson, D. & Kundys, D. O. Lightinduced size changes in BiFeO3 crystals. Nat. Mater. 9, 803–805 (2010).
 68
Choi, T., Lee, S., Choi, Y., Kiryukhin, V. & Cheong, S.W. Switchable ferroelectric diode and photovoltaic effect in BiFeO3 . Science 324, 63–66 (2009).
 69
Ji, W., Yao, K. & Liang, Y. C. Bulk photovoltaic effect at visible wavelength in epitaxial ferroelectric BiFeO(3) thin films. Adv. Mater. 22, 1763 (2010).
 70
Grinberg, I. et al. Perovskites oxides for visiblelightadsorbing ferroelectric and photovoltaic materials. Nature 503, 509–512 (2013).
 71
Alexe, M. Local mapping of generation and recombination lifetime in BiFeO3 single crystals by scanning probe photoinduced transient spectroscopy. Nano Lett. 12, 2193–2198 (2012).
 72
Yuan, G. L. & Wang, J. L. Evidences for the depletion region induced by the polarization of ferroelectric semiconductors. Appl. Phys. Lett. 95, 252904–1–3 (2009).
 73
Qin, M., Yao, K. & Liang, Y. C. Photovoltaic mechanisms in ferroelectric thin films with the effects of the electrodes and interfaces. Appl. Phys. Lett. 95, 022912–1–4 (2009).
 74
Yi, H. T., Choi, T., Choi, S. G., Oh, Y. S. & Cheong, S.W. Mechanism of the switchable photovoltaic effect in ferroelectric BiFeO3 . Adv. Mater. 23, 3403 (2011).
 75
Sung, J. H. et al. Single ferroelectricdomain photovoltaic switch based on lateral BiFeO3 cells. NPG Asia Mater. 5, e38 (2013).
 76
Basu, S. R. et al. Photoconductivity in BiFeO3 thin films. Appl. Phys. Lett. 92, 091905 (2008).
 77
Nonaka, K., Akiyama, M., Hagio, T. & Takase, A. Bulk photovoltaic effect in reduced/Oxidized lead lanthanum titanate zirconate ceramics. Jpn J. Appl. Phys. 34, 2344 (1995).
 78
Won, C. J., Park, Y. A., Lee, K. D., Ryu, H. Y. & Hur, N. Diode and photocurrent effect in ferroelectric BaTiO3−δ . J. Appl. Phys. 109, 084108 (2011).
 79
Festl, H. G., Hertel, P., Krätzig, E. & von Baltz, R. Investigations of the photovoltaic tensor in doped LiNbO3 . Phys. Status Solidi 113, 157–164 (1982).
 80
Inoue, R. et al. Enhanced photovoltaic currents in strained Fedoped LiNbO3 films. Phys. Status Solidi A 212, 2968–2974 (2015).
 81
Peterson, G. E. Control of the susceptibility of lithium niobate to laserinduced refractive index changes. Appl. Phys. Lett. 19, 130 (1971).
 82
Zaldo, C. & Fridkin, V. Bulk photovoltaic effect of LiNbO3:Fe in the liquidhe temperature range. Ferroelectr. Lett. Sect. 18, 17–21 (1994).
 83
Fridkin, V. et al. The bulk photovoltaic effect in LiNbO3, crystals under xray synchrotron radiation. Ferroelectr. Lett. Sect. 16, 1–5 (1993).
 84
Nechache, R. et al. Photovoltaic properties of Bi2FeCrO6 epitaxial thin films. Appl. Phys. Lett. 98, 202902 (2011).
 85
Nechache, R. et al. Bandgap tuning of multiferroic oxide solar cells. Nat. Photon. 9, 61–67 (2014).
 86
Stoumpos, C. C., Malliakas, C. D. & Kanatzidis, M. G. Semiconducting Tin and Lead iodide perovskites with organic cations: phase transitions, high mobilities, and nearinfrared photoluminescent properties. Inorg. Chem. 52, 9019–9038 (2013).
 87
Stranks, S. D. et al. Electronhole diffusion lengths exceeding 1 micrometer in an organometal trihalide perovskite absorber. Science 342, 341–344 (2013).
 88
Green, M. A., HoBaillie, A. & Snaith, H. J. The emergence of perovskite solar cells. Nat. Photon. 8, 506–514 (2014).
 89
Weller, M. T., Weber, O. J., Henry, P. F., Di Pumpo, A. M. & Hansen, T. C. Complete structure and cation orientation in the perovskite photovoltaic methylammonium lead iodide between 100 and 352 K. Chem. Commun. 51, 4180–4183 (2015).
 90
Even, J., Pedesseau, L., Jancu, J.M. & Katan, C. Importance of spinorbit coupling in hybrid organic/inorganic perovskites for photovoltaic applications. J. Phys. Chem. Lett. 4, 2999–3005 (2013).
 91
Umari, P., Mosconi, E. & De Angelis, F. Relativistic GW calculations on CH3NH3PbI3 and CH3NH3SnI3 perovskites for solar cell applications. Sci. Rep. 4, 4467 (2014).
 92
Zheng, F., Tan, L. Z., Liu, S. & Rappe, A. M. Rashba spinorbit coupling enhanced carrier lifetime in CH3NH3PbI3 . Nano Lett. 15, 7794–7800 (2015).
 93
deQuilettes, D. W. et al. Impact of microstructure on local carrier lifetime in perovskite solar cells. Science 348, 683–686 (2015).
 94
Lee, M. M., Teuscher, J., Miyasaka, T., Murakami, T. N. & Snaith, H. J. Efficient hybrid solar cells based on mesosuperstructured organometal halide perovskites. Sci. 338, 643–647 (2012).
 95
Colella, S. et al. Elusive presence of chloride in mixed halide perovskite solar cells. J. Phys. Chem. Lett. 5, 3532–3538 (2014).
 96
Stoumpos, C. C. et al. Hybrid germanium iodide perovskite semiconductors: active lone pairs, structural distortions, direct and indirect energy gaps, and strong nonlinear optical properties. J. Am. Chem. Soc. 137, 6804–6819 (2015).
 97
Zhou, W., Deng, H., Yang, P. & Chu, J. Structural phase transition, narrow band gap, and roomtemperature ferromagnetism in [KNbO3]1x[BaNi1/2Nb1/2O3]x ferroelectrics. Appl. Phys. Lett. 105, 111904 (2014).
 98
Zhou, W., Deng, H., Yang, P. & Chu, J. Investigation of microstructural and optical properties of (K,Ba)(Ni,Nb)O3 thin films fabricated by pulsed laser deposition. Mater. Lett. 181, 178–181 (2016).
 99
Choi, W. S. et al. Wide bandgap tunability in complex transition metal oxides by sitespecific substitution. Nat. Commun. 3, 689 (2012).
 100
Flückiger, U. & Arend, H. On the preparation of pure, doped and reduced KNbO3 single crystals. J. Cryst. Growth 43, 406–416 (1978).
 101
Xue, D. & Siyuan, P. Z. Chemical bond and nonlinear optical effects of crystals. J. Shanghai Univ. 3, 172–174 (1999).
 102
Fu, H. & Cohen, R. E. Polarization rotation mechanism for ultrahigh electromechanical response in singlecrystal piezoelectrics. Nature 402, 281–283 (2000).
 103
Wang, F., Grinberg, I. & Rappe, A. M. Band gap engineering strategy via polarization rotation in perovskite ferroelectrics. Appl. Phys. Lett. 104, 152903 (2014).
 104
Kou, L., Zhang, Y., Li, C., Guo, W. & Chen, C. Localstraininduced charge carrier separation and electronic structure modulation in zigzag zno nanotubes: role of builtin polarization electric field. J. Phys. Chem. C 115, 2381–2385 (2011).
 105
Bera, T. K. et al. Soluble semiconductors AAsSe2 (A=Li, Na) with a directbandgap and strong second harmonic generation: a combined experimental and theoretical study. J. Am. Chem. Soc. 132, 3484–3495 (2010).
 106
Song, J.H., Freeman, A. J., Bera, T. K., Chung, I. & Kanatzidis, M. G. Firstprinciples prediction of an enhanced optical secondharmonic susceptibility of lowdimensional alkalimetal chalcogenides. Phys. Rev. B 79, 245203 (2009).
 107
Priyadarshi, S., Pierz, K. & Bieler, M. Alloptically induced ultrafast photocurrents: beyond the instantaneous coherent response. Phys. Rev. Lett. 109, 216601 (2012).
 108
Morimoto, T. & Nagaosa, N. Topological nature of nonlinear optical effects in solids. Sci. Adv. 2, e1501524 (2016).
 109
Morimoto, T. & Nagaosa, N. Topological aspects of nonlinear excitonic processes in noncentrosymmetric crystals. Preprint at http://arxiv.org/abs/1512.00549 (2015).
Acknowledgements
L.Z.T., F.Z., F.W. and A.M.R. were supported by the US Department of Energy (DOE), under grant DEFG0207ER46431. S.M.Y. was supported by a National Research Council Research Associateship Award at the US Naval Research Laboratory. S.L. acknowledges the support from the Carnegie Institution for Science. We acknowledge computational support from the NERSC of the DOE.
Author information
Affiliations
Corresponding author
Ethics declarations
Competing interests
The authors declare no conflict of interest.
Rights and permissions
This work is licensed under a Creative Commons Attribution 4.0 International License. The images or other third party material in this article are included in the article’s Creative Commons license, unless indicated otherwise in the credit line; if the material is not included under the Creative Commons license, users will need to obtain permission from the license holder to reproduce the material. To view a copy of this license, visit http://creativecommons.org/licenses/by/4.0/
About this article
Cite this article
Tan, L., Zheng, F., Young, S. et al. Shift current bulk photovoltaic effect in polar materials—hybrid and oxide perovskites and beyond. npj Comput Mater 2, 16026 (2016). https://doi.org/10.1038/npjcompumats.2016.26
Received:
Revised:
Accepted:
Published:
Further reading

Large Bulk Piezophotovoltaic Effect of Monolayer 2HMoS2
The Journal of Physical Chemistry Letters (2021)

Twodimensional Weyl points and nodal lines in pentagonal materials and their optical response
Nanoscale (2021)

A Design Principle for Polar Assemblies with C 3 ‐Sym Bowl‐Shaped π‐Conjugated Molecules
Angewandte Chemie (2021)

Topological Quantum Materials from the Viewpoint of Chemistry
Chemical Reviews (2021)

Evaluation of nanostructured BiZn0.5Ti0.5O3 thin films deposited by RF magnetron sputtering
Materials Science and Engineering: B (2021)